Microstructure and Mechanical Properties of ASTM A743 ... Microstructure and Mechanical Properties...
Embed Size (px)
Transcript of Microstructure and Mechanical Properties of ASTM A743 ... Microstructure and Mechanical Properties...
DOI: http://dx.doi.org/10.1590/1980-5373-MR-2017-0468 Materials Research. 2017; 20(6): 1622-1629 © 2017
Microstructure and Mechanical Properties of ASTM A743 CA6NM Steel Welded by FCAW Process
Rafael de Paula Silvaa*, Maria Ismenia Sodero Toledo Fariaa, Luiz Fernando Cursino Briet de Almeidaa,
Carlos Angelo Nunesa, Décio Vieiraa, Wanderlei Borges Júniora
Received: May 05, 2017; Accepted: August 09, 2017
CA6NM steel is widely used in the manufacture of hydraulic turbines metallic parts, due to its resistance to corrosion and cavitation damage, combined with good weldability and fatigue properties. However, welding of this type of steel is complex and to ensure a minimum residual stress after welding it is necessary perform a post welding heat treatment (PWHT) of the part. This study aims to analyze the effect of a PWHT on the microstructure and mechanical properties of CA6NM steel weld joint produced by the FCAW process and compare it with the characteristics of an as-welded joint. A martensitic microstructure has been present in both materials. However, the PWHT material has shown finely dispersed retained austenite, in an amount near 10 vol.%. Vickers microhardness values of all regions of PWHT welded joint present lower hardness values compared to those of the as-welded joint. Despite nearly identical toughness values of the weld metal from AW and PWHT samples, results of fracture analysis have shown distinct features in appearance of the fractures.
Keywords: martensitic stainless steel, ASTM A743 CA6NM, FCAW process.
CA6NM steel (ASTM A743A743M (1998)1) is as soft martensitic stainless steel used in several cast parts of hydraulic turbines. It is the most common metallic alloy used in the manufacture of this type of equipment, replacing -Mn steels by offering better resistance against corrosion and cavitation damage2.
The low-carbon Martensitic steels CA6NM is offset with the addition of nickel, whose purpose is to expand the austenitic field, Therefore, keep the potential and enable complete austenitization and also to temper with the formation of martensite. The mechanical properties and impact strength features of the material are improved1,2.
Welding is extensively used in the assembling and repair of components made of CA6NM steel. Typically, the resulting microstructure at room temperature consists of tempered martensite and it can contain small amounts of δ ferrite and retained austenite3. According to the literature2,4, retained austenite improves mechanical properties such as impact toughness while the presence of delta ferrite may deteriorate the impact properties and raises the ductile to brittle transition temperature5,6.
The reduction of the toughness, as well as the high residual stresses, can shorten the life of the pieceas well as accelerate the cavitation process. However, the completion of heat treatment is limited by manufacturing condition and the size of the structures, the treatment is typically made in large
ovens heated by the combustion of fossil fuels, which carries on air pollution and drastic effects on the environment6,7.
Post weld heat-treatment (PWHT) of this material is applied to ensure a minimum residual stress of the component and increase the toughness. Low toughness reduces the life of the piece and accelerates the process of cavitation as well7.
The objective of this work was to evaluate the possible gains obtained by the application of a stress relieve heat- treatment through evaluation of the microstructure and mechanical properties, specially Charpy V-Notch (CVN) toughness, of CA6NM steel welded joints produced by the Flux Cored Arc Weld (FCAW) process. The work was divided into three main parts: welding (process of preparation of the samples, the consumable and realization of welding), microstructural analysis (optical microscopy, SEM with EDS, macrography and XRD); and analysis of mechanical properties (impact testing, hardness testing).
2. Experimental Procedure
The steel plate used in this work was manufactured by Electro Steel Altona S.A. According to the manufacturer, the material was produced in an electric arc furnace, refined using an AOD furnace (Argon Oxygen Decarburization) and cast in sand molds as blocks of 300x400x45 mm dimensions. The blocks were then submitted to a heat treatment involving quenching and tempering to achieve the required mechanical
aEscola de Engenharia de Lorena, Universidade de São Paulo, Lorena, SP, Brazil
1623Microstructure and Mechanical Properties of ASTM A743 CA6NM Steel Welded by FCAW Process
properties. Table 1 presents the CA6NM chemical composition provided by the manufacturer which is in agreement with the ASTM standard1.
Table 1. CA6NM steel chemical composition (wt.%) according to ASTM vs. Chemical analysis provided by the manufacturer10.
Element Manufacturer (ALTONA) ASTM A 743/A
Carbon 0.02 0.06 max.
Manganese 0.77 1.00 max.
Silícon 0.47 1.00 max.
Chrome 12.08 11.5 – 14
Níckel 3.80 3.5 – 4.5
Molybdenum 0.46 0.4 – 1.0
Phosphor 0.04 0.04 max.
Sulfur 0.01 0.03 max.
Aluminum 0.01 ----------
The welding consumable was flux cored AWS E410NiMoT1-4-1 of 1.6 mm diameter which meets the ASME and AWS standard and specification 9 SFA 5.22. Table 2 presents the chemical composition of the weld metal.
Table 2. Specified chemical composition of the welding consumable from AWS E410NiMoT1-4-1 electrode.
Element Deposited weld metal Specified
Carbon 0.025 0.06
Manganese 0.36 1.0
Silícon 0.36 1.0
Chrome 11.99 11.0 – 12.5
Níckel 4.42 4.0 – 5.0
Molybdenum 0.50 0.40 – 0.70
Phosphor 0.009 0.04
Copper 0.03 0.75
Sulfur 0.010 0.03
The plate was cut into four strips of 97x300x45 (mm) which were then machined to make chamfers for X shaped welds, as shown in Figure 1. The welding process was the FCAW, using a multi-threaded electronic welding machine LINCOLN model POWERTEC 305 c PRO and torch to pre and post-heat. The shielding gas used was SG-AC-25, 75% Argon- 25%CO2.
The chamfered strips were pre heated to 100°C before welding to decrease the cooling rate of the welding joint, seeking to avoid the formation of harmful microstructures in the weld, which may cause cold cracks as well as to mitigate the generation of residual stresses. A ceramic backing was added on the opposite side of the joint to provide a high
Figure 1. Illustration of the size of the specimens prepared for welding.
quality root. The joint was produced using the position 3G upward, interpasses temperature, around 200° C, to not compromise the microstructure of weld region and, consequently, the mechanical properties. The temperature control interpasses were also made with the aid of a pyrometer and contact thermometer. interspersed between sides A and B, as shown in Figure 2. The table 3 shows technical parameters used during the weld of the steel.
Figure 2. Illustration of the sequence of weld passes, side A, side B, and root.
Two X shaped plate tests were prepared following the procedures of ASME IX (2013)8 one to be characterized in the "as-welded condition" (AW) and the other in the post weld heat-treated condition (PWHT). The two joints were X-ray tested and have not presented any detectable defects. The stress relief heat treatment was carried out according to ASME VIII Div. I (2004)9, temperature of 580° C for 8 hours. The PWHT hold time was chosen in order to be similar to a real large component stress relief treatment.
For analysis by optical microscopy, the samples were submitted to usual metallographic preparation procedures involving cutting; grinding, polishing and etching with Vilella reagent that consists in 5 g if picric acid, 2.5 ml of HCl and 90 ml of ethylic alcohol. The images were obtained in a Zeiss Axiovert 40MAT optical microscope. The analysis were focused on four regions of each joint as indicated in Figure 3, R (root), C (center), T (top) and Z (heat affected zone).
Silva et al.1624 Materials Research
Table 3. Specified weld parameters during the procedure.
Nº of passes
Energy (J/cm) Temp (ºC)
1 1.6 25.2 220 9.7 34355 100 3 9 305
4 1.6 25.3 225 12.1 28215 200 2 51 345
5 1.6 26 230 15.7 22895 160 2 14 350
6 1.6 25.6 225 15.3 22546 190 2 17 350
10 1.6 24.5 225 14.7 22544 160 2 17 335
11 1.6 24.5 225 12.5 26493 183 2 41 335
14 1.6 23.5 208 14.0 20927 174 2 17 320
2 1.6 24 225 15.6 20715 180 1 57 305
3 1.6 25 235 12.2 28949 180 2 50 345
7 1.6 25 228 11.1 30943 180 3 10 350
8 1.6 25 220 15.3 21515 166 2 13 340
9 1.6 25.2 225 12.3 27588 191 2 43 335
12 1.6 25.2 225 16.0 21326 158 2 6 335
13 1.6 25.2 225 17.2 19759 180 1 55 330
15 1.6 23.5 215 14.9 20368 149 2 9 320
Figure 3. Macrograph showing the cross-section of a weld joint and the regions from which optical microscopic analysis was carried out.
X-ray diffraction was used to check the phases present, mainly retained austenite. A PANalytical X'pert PRO MPD diffractometer was used, with Cu-Kα radiation; Ni filter 40 kV voltage; tube current of 30 mA; scan range of 10 ≤ 2θ ≤ 120; step of 0.02° and counting time of 20s. The